190 likes | 1.28k Vues
Review: Depletion Region Recombination Flat Quasi-Fermi Level (QFL) Requires rate limiting recombination is slow compared to thermal diffusion Assuming: k n ~k p = σ v , Flat QFL We get for recombination in the bulk at position x, Note, Vapp < 0 here
E N D
Review: Depletion Region Recombination Flat Quasi-Fermi Level (QFL) Requires rate limiting recombination is slow compared to thermal diffusion Assuming: kn~kp = σ v , Flat QFL We get for recombination in the bulk at position x, Note, Vapp < 0 here
Review: Depletion Region Recombination -Substitute definitions and divide top and bottom by
Review: Depletion Region Recombination Maximum occurs when n(x) = p(x)
New Material: Recall we desire UTOTAL Continue with Udr,max, recalling we want to solve for UTOTAL, as We need definition for n(x) and p(x) You can show that Nm = concentration of e- for max U, n(xm)=p(xm) Xm= position where n=nm In region 1, x<xm Exp (-) so n(x)<n(xm) More band bending In region 2, x>xm Exp (+) so n(x)>n(xm) Less band bending
Calculating UTOTAL: Back to Math Substituting in for n(x) and p(x)
Calculating UTOTAL For normally doped Si with Kn~Kp (assumed) UMAX is strongly peaked away from W, so we can extend the integral from W’ ∞.
Calculating UTOTAL After a change of variables, Recognizing that:
UTOTAL Substituting for UMAX , we obtain A = 2: There are e- s and h+s recombining. It is as if you lose half of the voltage to the other carrier.
UTOTAL: Everyone Does it Differently Note: Nate and Mary quote a different value.
Quasi-Neutral Region Ionized donor atoms neutralized by injection of electrons into CB. p(x) has not changed: before injection of electrons, p(w)<p(w’) despite flat bands Concentration gradient causing holes to diffuse away from W’ into the bulk. Need to understand Diffusion/Recombination/Generation equations Assume No Generation
Diffusion-Recombination Diffusion: Putting it together: Need Boundary Conditions
Diffusion-Recombination Assume no recombination in D.R. or at S.S.
Diffusion-Recombination After the math: You tell me.
Diffusion-Recombination We only have p(x), so lets take region where flux only due to holes: at x=W’ Evaluate at x=W’
Schockley-Read-Hall Trapped states can be caused by metal impurities, oxygen, or dopants
Schockley-Read-Hall LLI: Lower Level Injection of Electrons and holes from photons For n-type: HLI: Generate more electrons and holes than We had in our lattice:
Schockley-Read-Hall Assuming LLI of n-type Leaving us with :
Schockley-Read-Hall Solving yields: For HLI, same assumptions: HLI decays twice as slowly LLI: Wait for hole carriers to recombine HLI: hole & e- carriers must recombine twice as long